Germanium Compounds Containing Ge═E Double Bonds (E = S, Se, Te) as Single-Source Precursors for Germanium Chalcogenide Materials.
Kim, Hyo-Suk; Jung, Eun Ae; Han, Seong Ho; Han, Jeong Hwan; Park, Bo Keun; Kim, Chang Gyoun; Chung, Taek-Mo; Inorganic chemistry 56 (2017) 4084–4092; doi:10.1021/acs.inorgchem.6b02697

data_4345597
_publ_section_title
;
 Germanium Compounds Containing Ge&#x2550;E Double Bonds (E = S, Se, Te)
 as Single-Source Precursors for Germanium Chalcogenide Materials.
;
_journal_issue                   7
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4084
_journal_page_last               4092
_journal_paper_doi               10.1021/acs.inorgchem.6b02697
_journal_volume                  56
_journal_year                    2017
_chemical_formula_sum            'C12 H28 Ge N2 S3'
_chemical_formula_weight         369.13
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 106.793(1)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.8559(2)
_cell_length_b                   19.2355(4)
_cell_length_c                   12.1759(2)
_cell_measurement_reflns_used    9940
_cell_measurement_temperature    296(1)
_cell_measurement_theta_max      27.63
_cell_measurement_theta_min      2.75
_cell_volume                     1761.46(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(1)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0177
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4390
_diffrn_reflns_theta_full        28.39
_diffrn_reflns_theta_max         28.39
_diffrn_reflns_theta_min         2.04
_exptl_absorpt_coefficient_mu    2.083
_exptl_absorpt_correction_T_max  0.7592
_exptl_absorpt_correction_T_min  0.4476
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    1.392
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             776
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.44
_exptl_crystal_size_min          0.14
_refine_diff_density_max         0.283
_refine_diff_density_min         -0.207
_refine_diff_density_rms         0.046
_refine_ls_extinction_coef       0.0015(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.052
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     164
_refine_ls_number_reflns         4390
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.051
_refine_ls_R_factor_all          0.0312
_refine_ls_R_factor_gt           0.0228
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0288P)^2^+0.5337P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0572
_refine_ls_wR_factor_ref         0.0609
_reflns_number_gt                3743
_reflns_number_total             4390
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic6b02697_si_004.cif
_cod_data_source_block           20150828_0m
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/home/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_exptl_crystal_density_meas' value 'none' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        1761.46(6)
_cod_original_sg_symbol_H-M      P2(1)/n
_cod_database_code               4345597